Strain Rate Dependent Behavior and Modeling for ... 1696 S.M. Ibrahim et al. / Strain Rate Dependent
Embed Size (px)
Transcript of Strain Rate Dependent Behavior and Modeling for ... 1696 S.M. Ibrahim et al. / Strain Rate Dependent
Abstract This paper investigates the stress-strain characteristics of Hybrid fiber reinforced concrete (HFRC) composites under dynamic com-pression using Split Hopkinson Pressure Bar (SHPB) for strain rates in the range of 25 to 125 s-1. Three types of fibers hooked ended steel fibers, monofilament crimped polypropylene fibers and staple Kevlar fibers were used in the production of HFRC compo-sites. The influence of different fibers in HFRC composites on the failure mode, dynamic increase factor (DIF) of strength, toughness and strain are also studied. Degree of fragmentation of HFRC composite specimens increases with increase in the strain rate. Although the use of high percentage of steel fibers leads to the best performance but among the hybrid fiber combinations stud-ied, HFRC composites with relatively higher percentage of steel fibers and smaller percentage of polypropylene and Kevlar fibers seem to reflect the equally good synergistic effects of fibers under dynamic compression. A rate dependent analytical model is pro-posed for predicting complete stress-strain curves of HFRC com-posites. The model is based on a comprehensive fiber reinforcing index and complements well with the experimental results. Keywords Hybrid fibers; Concrete; FRC; SHPB; Strain rate; Toughness; Reinforcing index; Stress-strain curve; DIF.
Strain Rate Dependent Behavior and Modeling for Compression Response of Hybrid Fiber Reinforced Concrete
Hybrid fiber reinforced concrete (HFRC) composite is a mix of concrete matrix and fibers with dif-ferent material and geometric properties that results in synergistic and superior performance com-pared to the use of only one type of fibers in concrete composites. Strong and stiff fibers (e.g. steel fibers, Kevlar fibers) can restrain micro-crack growth, thus improving the concrete strength, where-as relatively flexible fibers (e.g. Polypropylene fibers, Polyethylene fibers, Polyvinyl alcohol) im-prove material toughness by stress transfer mechanisms over larger crack openings (Abadel et al.,
S.M. Ibrahim a Tarek H. Almusallam a Yousef A. Al-Salloum a Aref A. Abadel a Husain Abbas a* a MMB Chair of Research and Studies in Strengthening and Rehabilitation of Structures, Department of Civil Engi-neering, King Saud University, Riyadh 11421, Saudi Arabia. *Author email: email@example.com. http://dx.doi.org/10.1590/1679-78252717 Received 17.12.2015 In revised form 09.03.2016 Accepted 04.04.2016 Available online 12.04.2016
1696 S.M. Ibrahim et al. / Strain Rate Dependent Behavior and Modeling for Compression Response of Hybrid Fiber Reinforced Concrete
Latin American Journal of Solids and Structures 13 (2016) 1695-1715
2015; Almusallam et al., 2013; Almusallam et al., 2014; Bolander et al., 2008). Some of the obvious advantages of the HFRC composites in construction practices are improved homogeneity, better crack management, possibility of slender structural members (Almusallam et al., 2013, 2014; Yu et al., 2014; Markovic et al., 2006). However, to ensure a balance between ultimate strength and strain capacity, optimum volume/weight proportion of different fibers is desired (Ahmed et al., 2007). For static loading conditions, HFRC composites result in better energy absorbing properties compared with that of mono-fiber concrete composites (Chen et al., 1996; Abou El-Mal et al., 2015; Li, 2012). A new type of steel fiber with spiral shape, proposed recently (Xu et al., 2012a, 2012b), has been found to demonstrate larger displacement capacity and provide better bonding compared to hooked-end, deformed and corrugated fibers (Hao and Hao, 2013; Hao et al., 2016).
The impact response of FRC has been investigated in several studies. Banthia et al. (1994) re-ported that the polypropylene fibers experience dramatic changes in their properties under high rates of tensile loading. The increased sensitivity of the polypropylene fibers at high strain rate load-ing conditions was believed to be related to a more viscoelastic character of the polypropylene fibers than steel or carbon fibers. Zhang et al. (2005) and Mohammadi et al. (2009) found better crack resistance properties and enhanced energy absorbing capacity of HFRC composite structures against impact. On the basis of drop weight tests performed on steel-polypropylene HFRC, Komlos et al. (1995) and Song et al. (2005) reported positive role of polypropylene fibers in improving the impact resistance of HFRC. This improvement was mainly attributed to the increase the tensile strain capacity of the concrete in the plastic state due to the addition of polypropylene fibers. This was further confirmed by Maalej et al. (2005) for quasi-static tensile tests and by Zhang et al. (2007) for multiple impacts. Almusallam et al. (2013, 2014) highlighted the importance of geometrical proper-ties of fibers in improving the impact resistance of HFRC slabs containing steel, polypropylene and Kevlar fibers. Bindiganavile et al. (2001, 2002) reported the decrease in toughness of SFRC with an increase in the dynamic strain rate observed in drop weight impact tests. This was attributed to the fact that fiber fractures produce a significantly more brittle response in the SFRC as opposed to the fiber pullout mode that is highly energy absorbing, since fiber fractures were observed to occur more commonly at higher strain rates. Their conclusion was further validated by Lok et al. (2003) at even higher strain rates. They reported that the contribution of steel fibers to the toughness of concrete decreases as the strain rate increases. Hao et al. (2016) reported that the spiral steel fibers contrib-ute more significantly to the SFRC beams in dissipating the impact energy than hooked end steel fibers.
Several investigators have studied the dynamic compression response of fiber reinforced concrete (FRC) using Split Hopkinson Pressure Bar (SHPB). Based on tests conducted on steel fiber rein-forced concrete (SFRC), Wang et al. (2008) reported significant influence of steel fibers in the sof-tening region of stressstrain curve as compared to their contributions in the initial elastic modulus. Li and Xu (2003, 2009) observed the role of basalt fibers in causing considerable increase in the energy absorption and the deformation capacity of basalt fiber based geopolymeric concrete. Due to the low percentage of fibers, no notable enhancement in dynamic compressive strength was ob-served. Chen et al. (2009) performed tests on the polyvinyl alcohol (PVA) fiber reinforced ground granulated blast-furnace slag (GGBFS) concrete. The calculations were carried out using the meth-od given in Lok et al. (2002). It was observed that due to the PVA fiber bridging, the toughness of
S.M. Ibrahim et al. / Strain Rate Dependent Behavior and Modeling for Compression Response of Hybrid Fiber Reinforced Concrete 1697
Latin American Journal of Solids and Structures 13 (2016) 1695-1715
the concrete materials was significantly increased under dynamic compression. Based on tests con-ducted on SFRC, Rong et al. (2010) reported significant improvement in its toughness with increase in the fiber percentage as well as the strain rate however no appreciable change was observed in DIF (strength). Wang et al. (2011) reported the bridging effect of fibers in the failure of SFRC. The failure mode of fibrous specimens with highest fiber percentage was essentially a spalling type fail-ure of concrete. Moreover, the toughness energy was proportional to the fiber content under dynam-ic compression. Liu et al. (2012) investigated experimentally and numerically the comparative influ-ence of steel fibers and rubber fibers/particles in fiber reinforced concrete (FRC) composite on the dynamic compression. Incorporating rubber fibers/particles in the concrete mix in lieu of the fine aggregate resulted in a decrease in the dynamic compressive strength. However, the toughness of the rubber reinforced concrete increased for rubber content up to 10% and a further increase in rubber content caused a decrease in toughness. Zhigang et al. (2012) and Wang et al. (2012) con-ducted experiments on polyethylene and steel FRC composites. The HFRC composites performed better and had significant strain rate effect as compared to the SFRC. Wang et al. (2010) numeri-cally investigated the dynamic compression behavior of SFRC using finite element analysis. It was reported that the specimen failure was due the combined effect of pressure-dependent plastic hard-ening and damage softening.
Investigations on the modeling of rate dependent stress-strain behavior of HFRC and engineered cementitious composites are quite limited as compared to modeling of rate dependent behavior of plain concrete (Yang et al., 2015; Lu, 2014; Mohammed et al., 2015; Elsanadedy et al., 2011; Al-Salloum et al., 2014, 2015). Wang et al. (2008) studied the rate dependent stressstrain behavior of SFRC and proposed a model for stress-strain curve based on Weibull function (Weibull, 1951). A simple constitutive model for the DIF (strength) was obtained for GGBFS based concrete by Chen et al. (2013). The models were based on experiments conducted on GGBFS concrete for strain rate range of 10-5 to 188 s-1. Su et al. (2014) gave expressions of the DIF (strength) and DIF (critical strain) for ceramic fiber reinforced concrete. However, different equations for different percentage of ceramic fibers were given. Su and Xu (2013) investigated the stress-strain behavior of ceramic fibers reinforced concrete using 100 mm SHPB apparatus for strain rates of 20 to 130 s-1 range. A statis-tical damage model was proposed and the stress-strain curves were obtained for strain rate range of 28 to 62 s-1. Two different equations for calculating the DIF (strength) were given. DIF (strength) and DIF (toughness) models were give